Tips & Tricks
Like this document? Why not share!
Corner truncated inverted u slot ...
Master Rinaudo Marzo 09
Can ho emerald vien ngoc luc bao gi...
Email sent successfully!
Show related SlideShares at end
Jun 25, 2014
Comment goes here.
12 hours ago
Are you sure you want to
Your message goes here
Be the first to comment
Be the first to like this
Number of Embeds
No notes for slide
Transcript of "20120140506010"
1. International Journal of Advanced Research in Engineering and Technology (IJARET), ISSN 0976 – 6480(Print), ISSN 0976 – 6499(Online) Volume 5, Issue 6, June (2014), pp. 62-67 © IAEME 62 IMPROVE MICROSTRUCTURE OF ALUMINUM ALLOYS BY MODIFICATION Mustafa A. Rijab1 , Ali I. Al-Mosawi2 1 Technical Institute of Baquba, Mechanical Department, IRAQ 2 Free Consultation, Babylon, Hilla, IRAQ ABSTRACT It was found that the particle microstructure received, the fibrous shape, and thus the addition of the titanium is in part, leads to a partial modification of the micrstructure, and with the increase of this component be enough to get the full modification. The results also showed that the heat homogeneity leads to change the shape of the silicon particles fibrous into a spherical shape clearly through the process of homogenizing. The results showed that it is possible to improve the properties of aluminum - Silicon alloy resulting from industrial waste from factories, to become the alloy with good mechanical properties. Because of the weakness of these characteristics, in terms of high hardness and brittleness, with weakness in operability. And that the spherical shape of the silicon particles are obtained through five basic stages. Keywords: Improve, Industrial Waste, Heat Homogenizing, Modification. INTRODUCTION In many situations, like those in Iraq have gone through, when shortage of fresh Al happens, remelting of scrapped castings becomes unavoidable to obtain new castings. However, non homogenous microstructure and low mechanical properties are characteristic of these castings obtained by remelting, especially when the scrapped materials are made from modified alloys [1,2]. The eutectic morphology ranges from plate-like to lamellar like in as cast condition to a circular like after modification or rapid cooling . Aluminum casting alloys are gaining wide popularity, as they combine several attractive properties such as low density, high stiffness, good casting characteristics, as well as improved properties if the alloy microstructure is refined or modified. The effect of modification has been attributed to both affecting nucleation and Si morphology through prohibiting its growth . INTERNATIONAL JOURNAL OF ADVANCED RESEARCH IN ENGINEERING AND TECHNOLOGY (IJARET) ISSN 0976 - 6480 (Print) ISSN 0976 - 6499 (Online) Volume 5, Issue 6, June (2014), pp. 62-67 © IAEME: http://www.iaeme.com/IJARET.asp Journal Impact Factor (2014): 7.8273 (Calculated by GISI) www.jifactor.com IJARET © I A E M E
International Journal of Advanced Research in Engineering and Technology (IJARET), ISSN 0976 – 6480(Print), ISSN 0976 – 6499(Online) Volume 5, Issue 6, June (2014), pp. 62-67 © IAEME 63 When Al-Si alloys are solidified the eutectic silicon is seen to consist of coarse plates in the sharp edges. These are detrimental to the mechanical properties . Homogenization treatments, originally designed for Al-Si cast alloys, also has an effect on the Si particles morphology, as it changes their shape from lamellar to spheroid [6,7]. The addition of elements like Na, Sr, Sb, and Ti was found to induce an effect on the microstructure of the eutectic alloy depending on their addition procedure and amount. Both modes of refinement of (Ti) and modification of Na, Sr, Sb have an effect on microstructure, but in a rather different way, as the first control the nucleation rate rather than the morphology of the second phase [8,9]. Al-Si casting alloys are known for their good casting properties and a great number of researches have been conducted on their refining and/or modification to optimize its mechanical properties [4,10]. While modification alters the shape of the Si phase. Some other external factors like vibration or rapid solidification cause an alternation in the morphology of the Si eutectic [9, 10]. However, soon afterwards the effect of modification was found. Al-Si casting alloys are particularly of great importance as they offer good casting properties, good corrosion resistance, in addition to improved wear resistance [4,8]. However, the morphology of Si eutectic in these alloys is of great significance on controlling their properties, as it is usually grows in lamellar or fibrous or spheroidized form . EXPERIMENTAL PROCEDURE The experimental program of this work consisted of producing a number of castings (6) by remelting scrapped castings made of Al-12%Si alloy in a gas furnace. The melt was refined by adding Ti in the range (0.09-0.18)% Ti. The melt composition was controlled by adding fresh Al. the Ti was added in an elemental form, weighted and wrapped with Al foil. The Ti-wrapped in foil was laid in the bottom of an alumina crucible and the molten metal was poured over it. The whole melt was held afterwards for 20 min in the gas furnace for melt homogenization. The molten metal was poured at 590 °C in a preheated steel mould. The cast pieces were homogenized at 410 °C for different durations 20, 40, 60, 80, 100, hrs. Composition %Alloy AlSnPbNiCrTiZnMgMnCuFeSi Rem.0.0030.0120.0050.0120.0450.0240.0050.1710.0210.2612Al-12%Si Rem.0.0040.0090.0040.0130.090.0250.0060.180.0200.2412 Al-12%Si- 0.09%Ti Rem.0.0040.0070.0040.0130.180.0260.0060.1780.0210.2512 Al-12%Si- 0.18%Ti RESULT AND DISCUSSIONS The depicted changes in microstructure reveals that the Si-eutectic changes its morphology by heating at 410°C through five stages; nucleation, fragmentation, spherodization, growth and
International Journal of Advanced Research in Engineering and Technology (IJARET), ISSN 0976 – 6480(Print), ISSN 0976 – 6499(Online) Volume 5, Issue 6, June (2014), pp. 62-67 © IAEME 64 finally stabilization. The first stage after (20) hrs. is a stage where growth of the Si starts by diffusion of Si from the matrix to the particles as shown in Fig.2. After (40) hrs. (see Fig.3) ,the Si starts to diffuse out of the Si-eutectic particles and fragmentation of these particles happens changing their morphology. After that the Si particles becomes spheroidized for both alloys without Ti and with 0.18%Ti, where as, only partial spherodization happens in the alloy containing 0.09%Ti. The spherodized particles start to grow, growth of the Si particles proceed with holding time till these grown particles reach a stable state of their size and changes only happen to their shape. The microstructure as of the Al-12%Si cast alloys without Ti and with 0.09%Ti & 0.18%Ti, respectively, is seen to consist of two phases mainly, which are primary α- Al and eutectic Si. Adding the 0.09%Ti is seeing to modify the Si-eutectic morphology slightly but has no effect on refining the primary(α). While, 0.18%Ti modifies the Si-eutectic morphology greatly and changes the primary (α) to have a fine dendritic structure. This effect is believed to be due to the role of Ti in reducing the melting point of the alloy, thus giving a higher chance for nucleation of the primaryα Al relative to the Si-eutectic, this is in turn refines the primary (α) phase and inhibits the Si growth. Fig.4, 5, 6 shown the microstructure of the studied alloys after homogenization at 410 °C for (60, 80, 100) hrs. respectively. It is a worth mentioning that recent references [3, 6] have pointed out that the addition of Titanium in various forms to aluminum Alloys have a strong effect on nucleating the primary aluminum phase. These studies have shown that Ti in solution in the liquid metal even below the 0.09% , determined by equilibrium data from the phase diagram, and as low as 0.09% would be expected to precipitate (TiAl3), which is an active nucleus for aluminum. The different surging times of heat treatment aims to detecting the changes that happens with the microstructure refinancing .It is worth noticing that the time necessary for stabilization changes from alloy to alloy, as stabilization happens after 100 hrs. for the alloy without Ti & with 0.18%Ti, while it happens after 100 hrs. for the alloy containing 0.09%Ti. This stable size of the Si-particles ranges from 5-11 µm. The measured hardness of all the studied alloys in as cast and homogenized conditions .The data shows that adding Ti to Al-Si eutectic cast alloys increase their hardness in as cast condition. This effect might be explained by an increase in the eutectic content or the formation of (TiSi) particles , which is not investigated in this study. Homogenization, of these alloys cause a significant drop in hardness of all alloys and this drop continues with homogenization time. The possible causes behind this drop in hardness are stress-relief and change in Si-eutectic morphology. However, these studies have recorded that (TiAl3) was present on (TiB2) crystals at the lower levels of Ti than that expected from the phase diagram (0.18%Ti) . Some of these studies reported a poisoning effect of Si on the grain refinement action of Ti when Si% is high due to the possibility of formation of TiSi . CONCLUSIONS 1. Adding elemental Ti (0.09%) to Al-12%Si alloy causes partial modification of the Si eutectic, and as Ti content reaches 0.18% maximum modification is gained. 2. Homogenization treatment of Al-12%Si cast alloys with or without Ti causes a modification in the Si eutectic morphology through 6 stages. 3. When Ti content reaches 0.18% the mechanisms for modification of Si eutectic through homogenization becomes similar to those of the alloy without Ti. 4. Adding Ti to Al-12%Si cast alloys causes an increase in their hardness. 5. The stabilization state is reached after (100) hrs. for the alloy with 0.09%Ti, while it is reached after (40) hrs. for the alloys without or with 0.18% Ti
International Journal of Advanced Research in Engineering and Technology (IJARET), ISSN 0976 – 6480(Print), ISSN 0976 – 6499(Online) Volume 5, Issue 6, June (2014), pp. 62-67 © IAEME 65 Fig.1: Microstructure of As Cast and Modified Alloys Fig.2: Microstructure of Homogenized Alloys with(20)hrs. At 410 °C Fig.3: Microstructure of Homogenized Alloys with (40)hrs. At 410 °C
International Journal of Advanced Research in Engineering and Technology (IJARET), ISSN 0976 – 6480(Print), ISSN 0976 – 6499(Online) Volume 5, Issue 6, June (2014), pp. 62-67 © IAEME 66 Fig.4: Microstructure of Homogenized Alloys with (60)hrs. At 410 °C Fig.5: Microstructure of Homogenized Alloys with (80)hrs. At 410 °C Fig.6: Microstructure of Homogenized Alloys with (100)hrs. At 410°C
International Journal of Advanced Research in Engineering and Technology (IJARET), ISSN 0976 – 6480(Print), ISSN 0976 – 6499(Online) Volume 5, Issue 6, June (2014), pp. 62-67 © IAEME 67 REFERENCES 1. S.F.Mustafa, 1995, “wear and wear Mechanisms of AL –20%Si/AL2O3 Composite”, part 2, wear, 155, P.77. 2. A. Somi Reddy, B.Npramila Bai, K.s.s Murthy and S.K.Biswas, 1998, “Mechanism of seizure of aluminum Silicon alloys sliding against steel”, wear, 181, P.658. 3. R.N. Grugel, 1999, “Evaluation of Primary Dendrite Trunk diameters in directionally Solidified AL-Si alloys”, Mater. Character. 18, P.313. 4. A sharma, 2008, “Heat Treatment: Principles and Techniques”, part 3, Prentice Hall of India, Private Ltd. 5. A.A.Das, 2011, “Some Observations on the effect of the pressure on the solidification of AL- Si eutectic alloys”, part 2, Brit. foundryman, 34, P.201. 6. S.Shivkumar, L.Wang and D.Apelian, 1991, “Molten Metal Processing of advanced cast aluminum alloys”, J. Met. Jan, P 26. 7. Y. Shimizu, y. Kato, S. Hashimoto and N.Tsuchiya, 1986, “Influence of phosphate and Sodium Halides on the structure of hyper eutectic AL-Si casting alloys ”, Aluminum, 62, P. 276. 8. A sharma, B.F. yilmaz, 2005, “Silicon crystals in aluminum – Silicon alloys”, Aluminum, part 3, P.338. 9. Metals Hand book, 2008, Vol.4, “Properties and Selection: Non ferrous alloys and pure metals”, part 2, American Society for Metals, Metals Part, Ohio. 10. R.A.Higgins, 2010, “Engineering Metallurgy, part 5, Applied physical Metallurgy”, Holder and Stoughton (London). 11. Dalip Kumar, Antariksha Verma and Sankalp Kulshrestha, “An Experimental Study of Wear Resistance of Al – Sic Coatings on Steel Substrate”, International Journal of Advanced Research in Engineering & Technology (IJARET), Volume 4, Issue 6, 2013, pp. 222 - 228, ISSN Print: 0976-6480, ISSN Online: 0976-6499. 12. Iessa Sabbe Moosa, “Powder Metallurgy and its Application in the Production of Permanent Magnets”, International Journal of Advanced Research in Engineering & Technology (IJARET), Volume 4, Issue 6, 2013, pp. 127 - 141, ISSN Print: 0976-6480, ISSN Online: 0976-6499. 13. Mohd Shadab Khan and Dr. Zahir Hasan, “Effect of Orientation and Applied Load on Abrasive Wear Property of Alumunium Alloy –Al6061”, International Journal of Mechanical Engineering & Technology (IJMET), Volume 4, Issue 4, 2013, pp. 89 - 96, ISSN Print: 0976 – 6340, ISSN Online: 0976 – 6359. 14. S. Soren, M. K. Banerjee, R. N. Gupta and N. Prasad, “Evolution of Microstructure in Microalloyed Steel under Continuous Cooling”, International Journal of Design and Manufacturing Technology (IJDMT), Volume 4, Issue 3, 2013, pp. 1 - 7, ISSN Print: 0976 – 6995, ISSN Online: 0976 – 7002. 15. R.Maguteeswarana, Dr. R.Sivasubramanian and V.Suresh, “Methodology Study and Analysis of Magnesium Alloy Metal Matrix Composites”, International Journal of Mechanical Engineering & Technology (IJMET), Volume 3, Issue 2, 2012, pp. 217 - 224, ISSN Print: 0976 – 6340, ISSN Online: 0976 – 6359.